BS ISO 20310:2018 pdf download – Thermal insulation for building equipment and industrial installations — Aluminosilicate wool products — Specification
This document specifies the classification，requirements and test methods for factory-madealuminosilicate wool products which are used for thermal insulation of industrial installations andbuilding equipment, for non-refractory applications.The products are delivered as blanket, module,felt, board, paper, textile and other forms.
This document describes product characteristics and testing methods, marking and labelling.
This document does not specify the required level of a given property to be achieved by a product todemonstrate fitness for purpose in a particular application.
The following documents are referred to in the text in such a way that some or all of their contentconstitutes requirements of this document. For dated references,only the edition cited applies. Forundated references, the latest edition of the referenced document (including any amendments) applies.ISO 836,Terminology for refractories
IS0 8302,Thermal insulation—Determination of steady-state thermal resistance and related properties —Guarded hot plate apparatus
ISO 8894-1，Refractory materials —Determination of thermal conductivity —Part 1: Hot-wire methods(cross-array and resistance thermometer)
ISo 9229, Thermal insulation -Vocabulary
ISO 10635,Refractory products — Methods of test for ceramic fibre products
ISO 13787,Thermal insulation products for building equipment and industrial installations 一Determination of declared thermal conductivity
ISO 29465, Thermal insulating products for building applications —Determination of length and width
3 Terms and definitions
For the purposes of this document, the terms and definitions given in ISO 9229,ISO 836 and thefollowing apply.
ISO and lEC maintain terminological databases for use in standardization at the following addresses:
-IEC Electropedia: available at http://www.electropedia.org/
– ISO online browsing platform: available at https://www.iso.org/obp
amorphous High Temperature Insulating Wool (HTIW) manufactured predominantly from molten raw minerals
Note 1 to entry: The main ingredients are Al 2 O 3 and SiO 2 , and may contain ZrO 2 and Cr 2 O 3 .
aluminosilicate wool (3.1) blanket formed into thick sections by needling, stacking or folding sheets,compressed to a higher density and typically supplied with integral anchoring systems
thin and flexible insulating material formed on a paper-making machine
4 Symbols and abbreviated terms
b width mm
d thickness mm
l length mm
d N nominal thickness of the product mm
λ thermal conductivity W/(m ⋅ K)
λ D declared thermal conductivity W/(m ⋅ K)
ρ a apparent density kg/m 3
ρ D nominal apparent density kg/m 3
4.2 Abbreviated terms
ITT initial type test
FPC factory production control
Product properties shall be tested in accordance with Clause 6. To comply with this document, products shall meet the requirements of 5.2 to 5.8, where applicable.
The test methods to be used for determination of each property are given in Table 5, which also shows the required test specimen dimensions and the minimum number of test specimens required to give one test result.
One test result for a product property is the average of the measured values on the number of test specimens given in Table 5.
For FPC, see Annex A.
Products shall be classified into one of six types according to the classification temperature per Table 1.
5.3 Permanent linear change Permanent linear change upon heating shall not be greater than 4,0 %. The test temperature shall be at the classification temperature as per Table 1.
5.4 Thermal conductivity The manufacturer shall make declaration for the thermal conductivity λ D . The table or curve of conductivity versus temperature (from 200 °C up to 1 100 °C, where applicable) shall be given according to ISO 13787. Thermal conductivity shall be based upon measurements carried out in accordance with ISO 8302 up to 800°C and shall be in accordance with ISO 8894-1 or ISO 10635 for temperatures above 800 °C.
5.5 Dimensions The length, l, and width, b, shall be determined in accordance with ISO 29465. The thickness, d, shall be determined in accordance with ISO 10635. No test result shall deviate from the nominal values by more than the tolerances given in Table 2.